 ```ADVANCED UNDERGRADUATE LABORATORY
EXPERIMENT 19
ELECTRICAL RESISTIVITY OF METALS
Last Revision:
Original By:
July 2005 by Jason Harlow
John Pitre
Theory
One of the prominent characteristics of metals compared with other solids such as insulators or
semiconductors, (see Experiment 20), is their high electrical conductivity, . This results from the large
number, n, of electrons per unit volume, typically n  5  1022 cm−3, corresponding to about 1 electron
per atom which is free to carry electric current.
For an applied electric field, E, the current density, J, is determined by n, the electric charge, e,
and the mass, m. We also need another quantity, the average time between collisions of the electron,
with thermally vibrating atoms or with impurities, which restore the electron to its average velocity
corresponding to zero applied field. We denote this time by Δt = 2, and call  the relaxation time. Thus
the average drift velocity v of the electrons in the field E is given by:
v  0 at
v  max

 a
2
2
where the magnitude of a is given by Newton’s 2nd Law:
F eE
a 
m m
so that
eE
v
(1)
m
and the magnitude of the current density is
ne 2
J  nev 
E
m
(2)
which, when compared with Ohm’s Law, J = E, gives
 
ne2
m
(3)
If we substitute the known values of n, e and m for a typical metal like copper, for which  = 0.6  106
Ω−1 cm−1 at room temperature, we obtain   2  10−14 s.
The relaxation time,, depends upon the amplitude of the thermal vibrations of the atoms, which
decreases with decreasing temperature, and also upon the concentration and nature of the impurities.
The probability of scattering per unit time, which is inversely proportional to the relaxation time,, is the
sum of probabilities of scattering by thermal vibrations and by impurities, so we can write
1


1
 ideal

1
 impurities
(4)
Since, from equation (3), the resistivity  = 1/  1/, we have
 = ideal + impurities = i + o
2
(5)
where their ideal resistivity, ρi, is that of a perfect single crystal sample with no impurities while o is
the resistivity contribution due to impurities.
One finds experimentally that ρi and o can be separated by measuring the temperature
dependence of the resistivity. As shown schematically in Figure 1, o is independent of temperature,
whereas ρi varies with temperature. D is the Debye temperature, the characteristic temperature of the
thermal vibrations of the crystal lattice. The value of D for several metals is given in Table 1. For
temperatures much lower than D, the ideal resistivity should vary as i(T)  T 5, where T is measured in
Kelvin. For temperatures much higher than D, i(T)  T.

i T
5
i T
0
T (K)
D (approx.)
Figure 1. Resistivity versus Temperature for a Normal Metal.
Debye
Superconducting
Temperature
Transition temperature
TC (K)
D (K)
Al
229
1.2
Cu
344
(does not superconduct)
In
109
3.4
Na
160
(does not superconduct)
Nb
252
9.2
Pb
96
7.2
Sn
195
3.7
W
270
0.01
Table 1. Debye temperatures and superconducting transition temperatures for some elements.
The normal boiling point of liquid helium, T = 4.2 K, is so far below D in most metals that,
unless the sample is extremely pure, the ideal resistivity is much less than the impurity resistivity.
Conversely, unless the sample is very impure, the ideal resistivity at room temperature is usually much
greater than the impurity resistivity. For this reason, the ratio of the resistivity at room temperature to its
3
value at 4.2 K, usually called the Residual Resistivity Ratio (R.R.R.) is often used as a measure of the
purity of the metal sample.

R.R.R.  RT
(6)
 4.2
The resistivity is related to the measured resistance by
RA

(7)
l
where l is the distance between potential leads and A is the cross sectional area. The temperature
relation between resistance and resistivity may be complicated if A and l vary appreciably as the
temperature changes. However, at low temperatures, thermal coefficients of expansion are low, so that
the change in dimensions from 4 K to 300 K is much less than the change in dimensions from 304 K to
600 K, for example. Also, for impurity estimation using R.R.R. measurements, one is only interested in
the order of magnitude of the R.R.R. value so that from equation (7) one can write
RRT
(8)
R4.2
Many metals become superconducting at low temperatures, with the resistivity falling abruptly to
zero at the superconducting temperature TC as is shown in Figure 2. Values for TC for several metals are
given in Table 1. Lead (Pb) has one of the highest values of TC for a metallic element, several degrees
above the normal boiling point of helium, so that its superconductivity can be readily demonstrated. For
a short explanation of the phenomenon of superconductivity, refer to Kittel's “Introduction to Solid State
Physics”, Chapter 12, or Chapter 34 of “Solid State Physics” by Ashcroft and Mermin.
R.R.R. 

0
TC
T (K)
Figure 2. Resistivity versus Temperature for a Superconductor.
There are other metals which display a resistance minimum at low temperatures as is shown in
Figure 3. Instead of flattening out or dropping to zero, the resistance increases strongly for temperatures
less than about 20 K (see Ashcroft and Mermin, p 688).
4

T (K)
Figure 3. Resistivity versus Temperature for alloys with a resistance minimum.
Experiment
The resistivities of three metal samples are to be measured from about 4.2 K to about 300 K.
There is a separate probe for each wire sample with the same pattern of connections in each case. The
wire samples are quite long, and are therefore wound into coils in order to make them more compact.
The different metal sample wires vary in length and wire thickness, so a comparison of their different
resistances does not necessarily reflect differences in resistivities.
The samples of pure Pb, pure Cu, and Au + 0.07% Fe are arranged with current and potential
leads as four terminal resistors for which the terminal connections are given in Figure 4. It is the
circular plug on the probe which carries the current and potential leads for the experimental sample.
green
voltage
2
4
1
5
white
3
red
current
black
Figure 4. Connections on the probe viewed facing the circular plug.
An alternating current is sent through the wire sample via the red and black connections. The
amplitude of this current can be made as constant as possible by connecting a large resistance in series
5
with the wire sample. You may use a decadal resistor and an ammeter to monitor the amplitude of the
current through the wire sample. By adjusting the value of the resistance across the decadal resistor
during the experiment, the amplitude of the current can be kept constant as the temperature changes.
The voltage drop across the wire sample is monitored via the green and white connections, and this can
be used to determine resistance of the wire sample. The voltage drop may be quite small, so a Lock-in
amplifier is used to measure the voltage between the green and white wires. The voltage may be read
directly off the dial on the Lock-in amplifier, or monitored with the computer by connecting the output
of the Lock-in amplifier to the computer. A possible suggested circuit is shown in Figure 5.
Wavetek
AC Generator
Lock-In Amplifier
Ref.
IN
OUT
Computer
Channel 1
“Lock-in Volt”
Resistor
Probe
Ammeter A
red
Metal
coil
black
white
green
Figure 5. Suggested circuit diagram for the resistance measurements.
Temperature measurements are made using a silicon diode as a sensing element. Some technical
information on silicon diodes as cryogenic sensors is given in Appendix I. The temperature is obtained
by measuring the voltage developed across the diode for a given current supplied by the constant current
source. There are red and white leads coming from the square Jones plug which are connected as
voltage leads across the temperature sensing diode. Measuring the voltage across these leads and using
the calibration tables provided in Appendix II will give the temperature of the wire sample. For each
probe the resistance of the sample coil and the connections to the thermometer should be checked at
room temperature at the start of the experiment. The output of the thermometer may be monitored
directly by a computer. A suggested circuit diagram is shown in Figure 6.
6
Constant
DC current
supply
Probe
Temp.
Sensitive
Diode
red
Computer
Channel 2
“Temperature
voltage”
V
white
Figure 6. Suggested circuit diagram for temperature measurement.
The probe must be pre-cooled in a liquid nitrogen bath until all major bubbling has ceased before
it is lowered into the liquid helium dewar. As a check, a measurement at 77 K should be made. When
making this measurement, one should be careful not to use liquid nitrogen that has been sitting in a wide
neck dewar exposed to the atmosphere for a long time. Liquid nitrogen can become contaminated with
oxygen from the atmosphere and will not be at the boiling point of pure nitrogen but a little nearer to the
eutectic for liquid air which is a few degrees higher than 77 K. Practically, one should expect a
deviation from 77 K of no more than a fraction of a degree.
The lowest temperature is obtained by lowering the probe into the dewar containing liquid
helium at its normal boiling point of 4.2 K. This operation should be done with the help of a laboratory
supervisor or technician.
After making a measurement at 4.2 K, measurements may be made at higher temperatures by
raising the bottom of the probe out of the liquid helium and having it cooled just in the helium gas.
Greater height above the liquid will correspond to higher temperature. In a similar manner to that for
helium, you may use the gas over liquid nitrogen to obtain temperatures above 77 K. Measurements up
to room temperature may be made if the temperature can be raised slowly enough so that the coil and
diode may be assumed to be at the same temperature.
Analysis
You will obtain three R versus T curves which will look, more or less, like Figures 1, 2 and 3.
For Cu it would be desirable to take the sample in the probe above room temperature to obtain
resistivities for T ranging through the D value and also the coefficient of the linear temperature above
room temperature. However, heating up the probe can cause damage to the probes so we ask you to
“make do” with a room temperature value for the Cu resistivity. You should be able to confirm the T 5
dependence at low temperatures. For a discussion of the linear and T 5 dependencies of the resistivity
see Ashcroft and Mermin p. 525 and Dekker p. 292.
7
Determine the residual resistance ratio for two of the wire samples and estimate it for Pb. The
values you obtain should show the effect of the iron impurity in the gold and other unspecified
It is possible, (see Dekker p. 294, and, in greater detail, Chapter 4 of Meaden which is given in
Appendix III), to obtain a value of the Debye temperature, D from electrical resistance measurements
made in the low and high temperature regions. Calculate a value for D for the copper sample and
compare it with the value D = 344 K from specific heat measurements.
For the Au + 0.07% Fe sample you should obtain a clear indication of the resistance minimum
and you could try to obtain confirmation of the ln(T) dependence of the Kondo contribution to the
resistivity. For some explanation of the Kondo effect in increasing order of complexity read the
following:
 Kittel, pp. 598-600
 Ashcroft and Mermin, pp. 687-9
 Hurd, pp. 181-191 (includes a simple analysis based on Feynman diagrams).
A discussion of the effect that magnetic exchange interaction has on the specific heat of dilute
magnetic alloys is given in Appendix IV. This should provide some feeling for how the dilute magnetic
impurity produces relatively large effects. In Appendix V is a reprint of a paper by Daybell and Steyert
which gives an experimental review of how the Kondo effect appears in measurements of the magnetic
susceptibility, resistivity, specific heat and thermoelectric power.
REFERENCES
1. N.W. Ashcroft and N.D. Mermin, Solid State Physics, 1976. (QC 176 A83)
2. A.J. Dekker, Solid State Physics, 1957. (QD 931 D43)
3. C.M. Hurd, Electrons in Metals, 1975. (QC 176.8 E4H87)
4. C. Kittel, Introduction to Solid State Physics, 8th edition, 2004 (John Wiley and Sons). (QC 171 K5)
5. G.T. Meaden, Electrical Resistivity of Metals, 1965. (QC 611 M5)
6. H.J. Zeiger and G.W. Pratt, Magnetic Interactions in Solids, 1973. (QC 176.8 M3Z44)
8
```